Upload
others
View
14
Download
0
Embed Size (px)
Citation preview
Effect of Covalent Functionalizationon Young’s Modulus of a Single-WallCarbon Nanotube
Priyal H. Shah and Romesh C. Batra
Abstract Effective utilization of carbon nanotubes (CNTs) as reinforcements incomposites necessitates good interfacial bonding with the surround matrix mate-rial. The covalent functionalization of CNTs is an effective method to enhance thisbonding. However, covalent bonds introduced by a functional group may alter thepristine structure of the CNT and lower its mechanical properties. Here we studythe effect of hydrogen (–H), hydroxyl (–OH), carboxyl (–COOH), and amine(–NH2) functionalization on Young’s modulus of a single-wall CNT (SWCNT)using molecular mechanics (MM) simulations with the MM3 potential and thesoftware TINKER. Both pristine and functionalized SWCNTs have been deformedin simple tension. From the strain energy of deformation vs. the axial strain curves,the value of Young’s modulus has been derived as a function of the functionali-zation group and the amount of functionalization. It is found that Young’s modulusdecreases by about 30 % with 20 % of functionalization, the reduction is essen-tially proportional to the increase in the percentage of the functionalizationmaterial and is nearly the same for each of the four functional groups studied.
Keywords Carbon nanotubes � Young’s modulus � Functionalization �Molecularmechanics � Virtual tension test
P. H. Shah � R. C. Batra (&)Department of Engineering Science and Mechanics, Virginia Polytechnic Instituteand State University, Blacksburg, VA 24061, USAe-mail: [email protected]
P. H. Shahe-mail: [email protected]
K. I. Tserpes and N. Silvestre (eds.), Modeling of Carbon Nanotubes, Grapheneand their Composites, Springer Series in Materials Science 188,DOI: 10.1007/978-3-319-01201-8_4, � Springer International Publishing Switzerland 2014
111
1 Introduction
Researchers have employed experimental, analytical, density functional theory(DFT), molecular dynamics (MD) and molecular mechanics (MM) simulations topredict mechanical properties of carbon nanotubes (CNTs). Assuming that the wallthickness of a single-wall CNT (SWCNT) can be approximated as 0.34 nm, Treacyet al. (1996), Wong et al. (1997), and Krishnan et al. (1998) experimentallydetermined that Young’s modulus of a CNT is in terapascal (TPa) range. Xing et al.(2004) employed MD simulations to predict Young’s modulus of a SWCNT. Li andChou (2003) computed elastic properties of CNTs using a combined structuralmechanics and MM approach. Chang and Gao (2003) investigated size dependentelastic properties of SWCNTs through MM simulations. Sears and Batra (2004)determined the wall thickness, Young’s modulus, and Poisson’s ratio of CNTsusing MM simulation with the MM3 potential and the software TINKER. Theyassumed that the response of a SWCNT in simple tension is energetically equiv-alent to that of a thin cylinder made of an isotropic and homogeneous material.Furthermore, the wall thickness of the cylinder equals that of the SWCNT. Theyfound the wall thickness and Young’s modulus of a SWCNT to be 0.046 nm and7.26 TPa, respectively. Shen and Li (2004) used MM potential and energy equiv-alent principle to determine values of five elastic constants of a CNT assuming theCNT as a transversely isotropic material with the centroidal axis of the tube as theaxis of transverse isotropy. Batra and Sears (2007) proposed that the axis oftransverse isotropy of a CNT is a radial line rather than the centroidal axis. Bystudying with the MM simulations radial expansion of a SWCNT, they showed thatYoung’s modulus in the radial direction is about 1/4th of that in the axial direction.Gupta and Batra (2008), Batra and Gupta (2008) predicted the wall thickness andthe material moduli of a SWCNT by matching frequencies of bending, axial andtorsional vibrations as well as that of radial breathing modes of a free–free SWCNTwith those of the continuous cylinder of the same length and mean radius as theSWCNT. Wu et al. (2008) developed an atomistic based finite deformation shelltheory for a SWCNT and found its stiffness in tension, bending, and torsion.
The SWCNTs due to their cylindrical shape, large length to diameter ratio, andhigh specific properties are potential candidates as reinforcements in composites.However, the effectiveness of SWCNTs as reinforcements depends on their uni-form dispersion in and strong adhesion with the surrounding matrix. It has beenvery challenging to simultaneously meet these two requirements. The function-alization of SWCNTs appears to be an effective means of achieving good bondingbetween SWCNTs and the surrounding matrix. The surface properties of CNTscan be modified by either physical or chemical functionalization. The physicalfunctionalization is achieved by attaching noncovalent groups, such as polymer,peptides or surfactants to the nanotubes. It is advantageous since it does not alterthe pristine structure of nanotubes hence the mechanical properties of CNTs arenot affected. However, these functional groups are attached to nanotubes withweak van der Waals interactions resulting in low load transfer efficiency between
112 P. H. Shah and R. C. Batra
the nanotube and the matrix. In comparison, the chemical functionalizationinvolving the covalent attachment of functional groups to atoms of CNTs providesrelatively strong interfacial bonding between CNTs and the surrounding matrixthereby enhancing the load transfer efficiency. Haddon et al. used the nanotube-bound carboxylic acid groups for attaching long alkyl chains to SWCNTs viaamide linkages (Chen et al. 1998; Hamon et al. 1999; Niyogi et al. 2001) and viacarboxylate-ammonium salt ionic interactions (Chen et al. 2001). Khare et al.(2002) developed hydrogenated CNTs using electric discharge. Sun et al. showedthat the esterification of the carboxylic acid groups could also be used to func-tionalize and solubilize nanotubes of any length (Riggs et al. 2000; Sun et al. 2001;Fu et al. 2001). Wilson et al. illustrated the use of anilines to functionalizenanotubes (Sun et al. 2001). Grujicic et al. (2006) investigated the effect ofcovalent functionalization of triple-walled CNTs on the efficiency of matrix-nanotube load transfer. Their results reveal that the covalent functionalizationimproves the load transfer efficiency especially when loads are applied in adirection orthogonal to the axis of the CNT. Experimental works (Cooper et al.2002; Barber et al. 2003; Shofner et al. 2006; Buffa et al. 2007; Sun et al. 2008)have demonstrated the effectiveness of covalent functionalization in increasing theinterfacial bonding strength between CNTs and polymer chains.
Although chemical functionalization is effective in enhancing the binding ofCNTs with the surrounding matrix, it may damage the pristine structure of a CNTdue to the introduction of covalent bonds, and reduce the mechanical stiffness ofthe CNT. Much of the research work dealing with the determination of Young’smodulus and other elastic properties of CNTs has considered pristine CNTs. Sincethe covalently functionalized CNTs would be better candidates for reinforcementsin a composite than the pristine CNTs, it is important to determine the effect ofcovalent functionalization on Young’s modulus of a CNT. Zhang et al. (2008) usedatomistic simulations to analyze mechanical properties of hydrogenated SWCNTsand found a decrease in Young’s modulus, strength, and ductility of the CNTs withan increase in the percentage of C–H bonds. Kuang and He (2009) computedYoung’s moduli of vinyl functionalized SWCNTs using MM simulations with thecondense-phase optimized molecular potential for atomistic simulation studies(COMPASS) force field and found that Young’s modulus depends on the densityof the sp3 hybridized carbon atoms and chirality of the CNTs. Up to 33 %reduction in Young’s modulus was observed in their study with 38 % content ofthe functionalizing material. Ling et al. (2012) predicted Young’s modulus offunctionalized CNTs using MM and MD simulations with the COMPASS forcefield and observed that Young’s modulus depends on the type of functionalizingmaterial and the amount of functionalization. Recently, Milowska and Majewski(2013) studied effect of different functional groups on elastic properties of func-tionalized CNTs using DFT calculations. Their results showed that an increase inamount of covalently bound material to the wall of a CNT decreases Young’s,shear and bulk moduli. Here we have considered four functional groups namely,hydrogen (–H), hydroxyl (–OH), carboxyl (–COOH), and amine (–NH2) andcompared their effects on the modulus of elasticity of a SWCNT with varying
Effect of Covalent Functionalization on Young’s Modulus 113
percentage of functionalization. The study has been carried out using MM simu-lations with the freely available software TINKER (Ponder 2000).
2 Molecular Mechanics Simulations
2.1 Force-Field
The MM3 potential (Allinger et al. 1989) with higher order expansions and cross-terms has been used to model interatomic interactions. This potential is suitable forstudying deformations of CNTs because of similarities between sp2 bonds in thehexagonal structure of CNTs and the hexagonal structure of aromatic proteins forwhich the potential was originally developed. This potential describes the energyof the system as summation of the energies due to bonded and non-bondedinteractions. The contributions for bonded interactions come from bond stretchingðUsÞ; in-plane angle bending ðUhÞ; out of plane bending ðUcÞ; torsion ðU/Þ; andcross-interactions including stretch-bend ðUsbÞ; angle–angle ðUhh0 Þ and stretch-torsion ðUs/Þ. The non-bonded interactions are van der Waals ðUvdWÞ and dipole–dipole electrostatic ðUll0 Þ. Equation (1) gives expressions for these energies.
Us ¼ 71:94Ksðr � r0Þ2½1� 2:55ðr � r0Þ þ7
122:552ðr � r0Þ2�
Uh ¼ 0:0219Khðh� h0Þ2 � ½1� 0:014ðh� h0Þ þ 5:6ð10�5Þðh� h0Þ2
� 7:0ð10�7Þðh� h0Þ3 þ 2:2ð10�8Þðh� h0Þ4�Uc ¼ 0:0219Kcc
2 � ½1� 0:014cþ 5:6ð10�5Þc2 � 7:0ð10�7Þc3 þ 2:2ð10�8Þc4�U/ ¼ V1=2ð Þ 1 þ cos /ð Þ þ V2=2ð Þ 1 þ cos 2/ð Þ V3=2ð Þ 1 þ cos 3/ð ÞUsh ¼ 2:511Ksh½ðr � r0Þ þ ðr0 � r00Þ�ðh� h0Þ
Uhh0 ¼ �0:021914Khh0 h � h0ð Þ h0 � h00� �
Us/ ¼ �5:9975Ks/ðr � r0Þð1þ cos 3/Þ
UvdW ¼ e �2:25 rv=rð Þ6þ 1:84 105� �
exp �12:00 rv=rð Þf gh i
Ull0 ¼14:3928½ll0ðcos v� 3 cos a cos a0Þ�
R3Dð1Þ
Parameters r, h and / in Eq. (1) are shown in Fig. 1. Variable c is the anglebetween the plane and one of the bonds. A subscript, 0, on a variable represents itsvalue in the configuration of minimum potential energy. Variables l and l0arebond centered dipole moments, v is the angle between two dipoles, a and a0 areangles made by two dipoles with the line connecting their centers, and R is thedistance between their centers. The values of constants Ks, Kh, Kc; K 0hh;V1;V2;
V3;Ksh;Ks/; e; rvand D given by Ponder (2000) are used in this work.
114 P. H. Shah and R. C. Batra
2.2 Modeling of Functionalized SWCNTs
Functionalization of a zigzag (10, 0) finite length SWCNT of aspect ratio 12 hasbeen considered as a model problem. The molecular structure of a functionalizedSWCNT can be obtained from topologies of the pristine SWCNT and the func-tional group. In order to obtain the relaxed configuration of the SWCNT weminimize its potential energy by using the steepest decent algorithm with the rootmean square (rms) gradient of 0.001. The diameter and the length of the relaxedtube are found to be 7.44 Å and 87.75 Å, respectively. The functional group is thenpositioned adjacent to a carbon atom of the relaxed CNT and the potential energyof the structure is minimized to obtain the relaxed configuration of the function-alized CNT. Note that the introduction of covalent bonds at the functional sitesalters the hybridization of the affected carbon atoms from sp2 to sp3. The per-centage of functionalization is defined as the ratio of the number of carbon atomsto which atoms of a functional group are attached to the total number of carbonatoms in the CNT. Four different functionalized CNTs have been studied withhydrogen, hydroxyl, carboxyl, and amine as the functionalizing groups. The car-bon atoms to which a functional group is attached are randomly selected but thesame set of atoms is used in each of the functionalized CNT for maintainingconsistency in the numerical experiments. Figure 2 depicts schematics of thefunctional groups attached to a carbon atom of the CNT. The atoms in white, red,and blue color represent hydrogen, oxygen, and nitrogen atoms, respectively. Itshould be clear from sketches displayed in the figure that the covalent bondbetween the carbon atom and a functional group pulls out the carbon atom radiallyresulting in the distortion of the CNT at the functional site. The SWCNTs func-tionalized with these groups are schematically shown in Fig. 3.
2.3 Virtual Simple Tension Experiments
While conducting virtual tension tests on the pristine and the functionalizedSWCNT, its ends are left open and not saturated with hydrogen atoms which maychange the bonding structure at the ends and lead to end effects. Furthermore,carbon atoms one diameter away from each end are fixed during simulations. The
Fig. 1 Definitions of threemolecular mechanicsvariables (Sears and Batra2004)
Effect of Covalent Functionalization on Young’s Modulus 115
nanotubes are gradually deformed in tension and compression by a total of 3 %axial strain. After each displacement increment applied to atoms near the end faces,the tubes are allowed to equilibrate by minimizing their potential energies. Theenergy required to deform the tube equals its strain energy. The strain energydensity is computed by dividing the strain energy by the volume of the CNT whichis taken equal to that of a continuum cylinder of length and diameter equal to those
Fig. 2 Schematics of acarbon atom of the CNTattached with a hydrogen(–H) b hydroxyl (–OH),c carboxyl (–COOH), andd amine (–NH2) groups
116 P. H. Shah and R. C. Batra
of the relaxed pristine SWCNT and thickness equal to 0.34 nm. A polynomialthrough the data points is fitted by the least squares method. The first and the secondderivatives of the strain energy density with respect to the axial strain yield thecorresponding axial stress and Young’s modulus, respectively. This procedure is thesame as that used by Sears and Batra (2004) to find Young’s modulus of a SWCNT.
3 Numerical Results
3.1 Validation of the Functionalization
In the relaxed configuration of the functionalized CNTs, the equilibrium bondlength between the carbon atoms of the CNT and the adjoining atoms of thefunctional group, if present, has been computed from the equilibrated configura-tions. The C–H bond length in the hydrogen functionalized CNT is found to be1.11, which agrees well with that (1.11) in the modified orthogonal tight bindingmodel (Volpe and Cleri 2003) as well as the 1.12 given by the DFT calculations(Letardi et al. 2002). Methanol (CH3OH), acetic acid (CH3COOH), and amino
Fig. 3 Schematics of a (10, 0) SWCNT functionalized with 20 % a hydrogen (–H), b hydroxyl(–OH), c carboxyl (–COOH), and d amine (–NH2) groups
Effect of Covalent Functionalization on Young’s Modulus 117
methane (CH3NH2) are simple structures representing covalent bonds between asp3 hybridized carbon and hydroxyl, carboxyl, and amine functional group,respectively. These structures can be generated using simplified molecular-inputline-entry system (SMILES) specification (Weininger 1988; Weininger et al. 1989)as shown in Fig. 4. In order to validate the functionalization of the CNTs withhydroxyl, carboxyl, and amine groups, the bond angles and bond lengths of thefunctional groups in the relaxed configuration of the functionalized CNTs havebeen measured and compared with those in methanol, acetic acid and aminomethane. In Tables 1, 2 and 3, we have listed values of these parameters forhydroxyl, carboxyl, and amine groups, respectively. It is evident that there is goodagreement between the two sets of values.
3.2 Analysis of Relaxed Configurations
The number of iterations required in the steepest descent method to minimizepotential energies of –H, –OH, –COOH and –NH2 functionalized CNTs is plotted
Table 2 Values of geometricparameters in the carboxylgroup
Acetic acid CNT–COOH
C–O–H angle (degrees) 107.39 107.6R–C–O angle (degrees) 112.04 111.89R–C = O angle (degrees) 126.04 126.27C–O length (Å) 1.35 1.35C = O length (Å) 1.2 1.21O–H length (Å) 0.97 0.97R–C length (Å) 1.5 1.53
Note R denotes sp3 hybridized carbon atom
Fig. 4 Structures ofa methanol, b acetic acid, andc amino methane generatedusing SMILES
Table 1 Values ofgeometric parameters in thehydroxyl group
Methanol CNT–OH
R–O–H angle (degrees) 108.13 109.18R–O length (Å) 1.43 1.43O–H length (Å) 0.95 0.95
Note R denotes sp3 hybridized carbon atom
118 P. H. Shah and R. C. Batra
in Figs. 5a, b and 6a, b respectively. Note that 0 % functionalization represents thepristine CNT. It can be observed from results depicted in Fig. 5a that when theCNT is functionalized with hydrogen, the potential energy of the relaxed func-tionalized structure is less than that of the relaxed pristine CNT, and this differenceincreases with an increase in the percentage of functionalization. It is because thefunctionalization breaks the pi-bond of the sp3 hybridized carbon atoms andchanges the atom type from alkene to the more stable alkane. Similar character-istics are observed with the hydroxyl and the amine functionalization while thepotential energy curves for the carboxyl functionalized CNTs do not exhibit thesame behavior due to the presence of double bonds in the –COOH group.
In Fig. 7a we have presented the contribution from each energy term of theMM3 potential to the total potential energies of the pristine CNT for the hydrogenfunctionalized CNTs in their relaxed configurations. These have been normalizedwith respect to corresponding energies of the relaxed pristine CNT.
It can be observed from results included in the figure that the sum of theenergies associated with the torsional and Van der Waals interactions are about90 % of the total potential energy of the pristine CNT. The functionalizationreduces these components of energies, thereby reducing the total potential energyand the reduction increases with an increase in the percentage of functionalization.Similar results for hydroxyl, carboxyl and amine functionalized CNTs are pre-sented in Figs. 7a, b and 8a, b. Here, small effect of the electrostatic interactionshas been observed on the total potential energies of the CNTs because of thepresence of dipole moments in these functional groups. For the carboxyl func-tionalized SWCNT, the potential energy is not a monotonically increasing functionof the amount of functionalization.
3.3 Results from Virtual Experiments
In the calculation of Young’s modulus, as stated above, the thickness of a SWCNTis assumed to be 0.34 nm. The variation of the computed strain energy densitywith the axial strain for the pristine CNT is shown in Fig. 9. The third orderpolynomial fit to the strain energy density of the pristine CNT vs. the axial straindata with the regression coefficient of 1.0 is
Table 3 Values of geometricparameters in the aminegroup
Amino methane CNT–NH2
H–N–H bond angle (degrees) 106.35 106.09R–N–H bond angle (degrees) 112.35 113.29Dihedral angle between
two R–N–H planes119.78 121.38
N–H bond length (Å) 1.01 1.01R–N bond length (Å) 1.46 1.46
Note R denotes sp3 hybridized carbon atom
Effect of Covalent Functionalization on Young’s Modulus 119
Wv ¼ �7:46 1011� �
e3 þ 5:03 1011� �
e2 þ 5:62 105� �
e ð2Þ
where Wv is the strain energy density in J/m3 and e is the nominal axial strain.Thus, expressions for the axial stress and the modulus of elasticity E in Pa are
r ¼ �2:24 1012� �
e2 þ 1:101 1012� �
e þ 5:62 105� �
ð3Þ
E ¼ �4:48 1012� �
e þ 1:01 1012� �
ð4Þ
Fig. 5 For four different percentages of functionalization, minimization of the potential energiesof a SWCNT functionalized with a –H, b –OH
120 P. H. Shah and R. C. Batra
The modulus of elasticity at zero axial strain equals 1.01 TPa. It compares wellwith that reported in the literature (Treacy et al. 1996; Wong et al. 1997; Krishnanet al. 1998). For the hydrogen functionalized CNT, the strain energy vs. the axialstrain variation and the axial stress-axial strain curves for different percentages offunctionalization are shown in Fig. 10a, b, respectively.
Fig. 6 For four different percentages of functionalization, minimization of the potential energiesof a SWCNT the functionalized with a –COOH, and b –NH2 groups
Effect of Covalent Functionalization on Young’s Modulus 121
In computing the strain energy density, the volume of the functionalized CNT istaken equal to that of the pristine CNT. These plots reveal that the functionali-zation reduces the strain energy of deformation, and the slope (hence the modulusof elasticity) of the stress–strain curve for the functionalized tube is less than that
Fig. 7 Break down of total potential energy, U, in the individual energy components for therelaxed configurations of a hydrogen, b hydroxyl, functionalized CNTs with percentage offunctionalization varying from 0 to 20 %
122 P. H. Shah and R. C. Batra
of the pristine tube. Moreover, the modulus of elasticity decreases with an increasein the percentage of functionalization. This reduction in the modulus of elasticitycould be due to the non-uniformities in the nanotube structure introduced by the
Fig. 8 Break down of total potential energy, U, in the individual energy components for therelaxed configurations of a carboxyl, and b amine functionalized CNTs with percentage offunctionalization varying from 0 to 20 %
Effect of Covalent Functionalization on Young’s Modulus 123
functionalization that lead to localized deformation at the functional sites. Similarresults for hydroxyl, carboxyl, and amine groups are exhibited in Figs. 11, 12 and13, respectively.
Values of Young’s modulus of the functionalized CNTs for different percent-ages of functionalization listed in Table 4 suggest that they do not depend muchupon the functionalization agent.
In Table 5, we have summarized similar results reported in the literatureobtained using various computational methods and force fields along with themajor results of the present study. It should be clear from the summary provided inTable 5 that the present results agree with those of other researchers. To betterunderstand the effect of functionalization on Young’s modulus, the strain energiesof the deformation in the tension tests of the pristine and the functionalized CNTshave been obtained in terms of their bonded and non-bonded energy components.In Figs. 14a, b and 15a, b we have depicted the contribution of individual energyterms to the total reduction in the strain energy of deformation due to hydrogen,hydroxyl, carboxyl, and amine functionalization, respectively. These values havebeen normalized with respect to those of the pristine CNT. These results indicatethat the functionalization reduces the strain energies associated with bond-stretching and angle bending and increases the strain energies due to torsional,stretch-bend, and van der Waals interactions. The resulting effect is net reductionin strain energy and the reduction is proportional to the amount of functionalizingmaterial attached to the wall of the CNT. Various components of the strain energyfor 20 % of functionalization are plotted in Fig. 16. It can be concluded from theseresults that the type of functional group is found to have significant effect on strain
Fig. 9 Strain energy density of the pristine SWCNT vs. the axial strain computed using theMM3 potential
124 P. H. Shah and R. C. Batra
Fig. 10 a Variation of the strain energy per atom with axial strain, and b axial stress-axial straincurves of –H functionalized SWCNT with the percentage of functionalization varied from 5 to20 %
Effect of Covalent Functionalization on Young’s Modulus 125
Fig. 11 a Variation of the strain energy per atom with axial strain, and b axial stress-axial straincurves of –OH functionalized SWCNT with the percentage of functionalization varied from 5 to20 %
126 P. H. Shah and R. C. Batra
Fig. 12 a Variation of the strain energy per atom with axial strain, and b axial stress-axial straincurves of –COOH functionalized SWCNT with the percentage of functionalization varied from 5to 20 %
Effect of Covalent Functionalization on Young’s Modulus 127
Fig. 13 a Variation of the strain energy per atom with axial strain, and b axial stress-axialstrain curves of –NH2 functionalized SWCNT with the percentage of functionalization variedfrom 5 to 20 %
Table 4 Young’s modulus of the SWCNT functionalized with different groups
Modulus of elasticity (TPa)
% of functionalization With hydrogen With hydroxyl With carboxyl With amine
0 1.01 1.01 1.01 1.015 0.91 0.91 0.91 0.91
10 0.82 0.81 0.80 0.8215 0.76 0.75 0.72 0.7420 0.70 0.69 0.67 0.66
Note 0 % functionalization represents the pristine CNT
128 P. H. Shah and R. C. Batra
Tab
le5
Sum
mar
yof
theo
reti
cal
pred
icti
ons
ofre
duct
ion
inY
oung
’sm
odul
usof
SW
CN
Ts
wit
hco
vale
ntfu
ncti
onal
izat
ion
Ana
lysi
sm
etho
dP
oten
tial
/for
cefi
eld
CN
TF
unct
iona
lgr
oup
Per
cent
age
offu
ncti
onal
izat
ion
Per
cent
age
redu
ctio
nin
You
ng’s
mod
ulus
Ref
eren
ce
MM
MM
3(1
0,0)
–H5
10P
rese
ntst
udy
1019
–OH
510
1020
–CO
OH
510
1021
–NH
25
1010
19A
FE
M2n
dge
nera
tion
inte
rato
mic
(9,
0)–H
106
Zha
nget
al.
(200
8)20
12M
MC
OM
PA
SS
(10,
0)–C
2H
38
16K
uang
and
He
(200
9)21
31M
DC
OM
PA
SS
(10,
10)
–H5
11L
ing
etal
.(2
012)
–OH
516
–CO
OH
515
–NH
25
14D
FT
–(1
0,0)
–OH
69
Mil
owsk
aan
dM
ajew
ski
(201
3)10
12–C
OO
H6
910
14–N
H2
69
1012
Effect of Covalent Functionalization on Young’s Modulus 129
Fig. 14 Break down of the total strain energy of deformation into the individual energycomponents for a hydrogen, b hydroxyl, functionalized CNTs with percentage of functional-ization varying from 0 to 20 %
130 P. H. Shah and R. C. Batra
Fig. 15 Break down of the total strain energy of deformation into the individual energycomponents for a carboxyl, and b amine functionalized CNTs with percentage of functional-ization varying from 0 to 20 %
Effect of Covalent Functionalization on Young’s Modulus 131
energies associated with bond stretching and bond angle bending compared toother energy components but the same net effect is obtained for all functionalgroups considered here.
4 Conclusions
We have studied the effect of covalent functionalization on Young’s modulus of aSWCNT. The functionalization localizes deformations of the CNT at the func-tionalized sites, which decreases the modulus of elasticity and this reductionincreases with an increase in the percentage of functionalization. The type offunctional group is found to have negligible effect on the value of Young’smodulus of the functionalized SWCNT. Approximately 30 % reduction in thevalue of Young’s modulus of the pristine CNT occurs for 20 % offunctionalization.
Acknowledgments This research was sponsored by the Army Research Laboratory and wasaccomplished under Cooperative Agreement Number W911NF-06-2-0014. The views and con-clusions contained in this document are those of the authors and should not be interpreted asrepresenting the official policies, either expressed or implied, of the Army Research Laboratory orthe U.S. Government. The U.S. Government is authorized to reproduce and distribute reprints forGovernment purposes notwithstanding any copyright notation hereon.
Fig. 16 Break down of the total strain energy of deformation into the individual energycomponents for the CNTs functionalized (20 %) with different functional groups
132 P. H. Shah and R. C. Batra
References
Treacy MMJ, Ebesen TW, Gibson JM (1996) Exceptionally high Young’s modulus observed forindividual carbon nanotubes. Nature (London) 381:678–680
Wong EW, Sheehan PE, Lieber CM (1997) Nanobeam mechanics: elasticity, strength andtoughness of nanorods and nanotubes. Science 277:1971–1975
Krishnan A, Dujardin E, Ebbesen TW, Yianilos PN, Treacy MMJ (1998) Young’s modulus ofsingle-walled nanotubes. Phys Rev B 58:14013–14019
Xing BW, Chun ZC, Zhao CW (2004) Simulation of Young’s modulus of single-walled carbonnanotubes by molecular dynamics. Physica B 352:156–163
Li C, Chou TW (2003) A structural mechanics approach for the analysis of carbon nanotubes. IntJ Solids Struct 40:2487–2499
Chang T, Gao H (2003) Size-dependent elastic properties of a single-walled carbon nanotube viaa molecular mechanics model. J Mech Phys Solids 51:1059–1074
Sears A, Batra RC (2004) Macroscopic properties of carbon nanotubes from molecular mechanicssimulations. Phys Rev B 69:Art. No. 235406
Shen L, Li J (2004) Transversely isotropic elastic properties of single-walled carbon nanotubes.Phys Rev B 69:045414
Batra RC, Sears A (2007) Uniform radial expansion/contraction of carbon nanotubes and theirtransverse elastic moduli. Modell Simul Mater Sci Eng 15:835–844
Gupta SS, Batra RC (2008) Continuum structures equivalent in normal mode vibrations to single-walled carbon nanotubes. Comput Mater Sci 43:715–723
Batra RC, Gupta SS (2008) Wall thickness and radial breathing modes of single-walled carbonnanotubes. ASME J Appl Mech 75:Art. No. 0610101
Wu J, Hwang KC, Huang YJ (2008) An atomistic-based finite-deformation shell theory forsingle-wall carbon nanotubes. J Mech Phys Solids 56:279–292
Chen J, Hamon MA, Hu H, Chen Y, Rao AM, Eklund PC, Haddon RC (1998) Solution propertiesof single-walled carbon nanotubes. Science 282:95–98
Hamon MA, Chen J, Hu H, Chen Y, Itkis ME, Rao AM, Eklund PC, Haddon RC (1999)Dissolution of single-walled carbon nanotubes. Adv Mater 11:834–840
Niyogi S, Hu H, Hamon MA, Bhowmik P, Zhao B, Rozenzhak SM, Chen J, Itkis ME, Meier MS,Haddon RC (2001) Chromatographic purification of soluble single walled carbon nanotubes(s-SWNTs). J Am Chem Soc 123:733–734
Chen J, Rao AM, Lyuksyutov S, Itkis ME, Hamon MA, Hu H, Cohn RW, Eklund PC, ColbertDT, Smalley RE, Haddon RC (2001) Dissolution of full-length single-walled carbonnanotubes. J Phys Chem B 105:2525–2528
Khare B, Meyyappan M, Cassell AM, Nguyen CV, Han J (2002) Functionalization of carbonnanotubes with atomic hydrogen from a glow discharge. Nano Lett 2:73–77
Riggs JE, Guo Z, Carroll DL, Sun YP (2000) Strong luminescence of solubilized carbonnanotubes. J Am Chem Soc 122:5879–5880
Sun YP, Huang W, Lin Y, Fu K, Kitaygorodskiy A, Riddle LA, Yu YJ, Carroll DL (2001a)Soluble dendron-functionalized carbon nanotubes: preparation, characterization, and proper-ties. Chem Mater 13:2864–2869
Fu K, Huang W, Lin Y, Riddle LA, Carroll DL, Sun YP (2001) Defunctionalization offunctionalized carbon nanotubes. Nano Lett 8:439–441
Sun Y, Wilson SR, Schuster DI (2001b) High dissolution and strong light emission of carbonnanotubes in aromatic amine solvents. J Am Chem Soc 123:5348–5349
Grujicic M, Sun YP, Koudela KL (2006) The effect of covalent functionalization of carbonnanotube reinforcements on the atomic-level mechanical properties of poly-vinyl-ester-epoxy.Appl Surf Sci 253:3009–3021
Cooper CA, Cohen SR, Barber AH, Daniel WH (2002) Detachment of nanotubes from a polymermatrix. Appl Phys Lett 81:3873–3875
Effect of Covalent Functionalization on Young’s Modulus 133
Barber AH, Cohen SR, Daniel WH (2003) Measurement of carbon nanotube-polymer interfacialstrength. Appl Phys Lett 82:4140–4142
Shofner ML, Khabashesku VN, Barrera EV (2006) Processing and mechanical properties offluorinated single-wall carbon nanotube–polyethylene composites. Chem Mater 18:906–9013
Buffa F, Abraham GA, Grady BP, Resasco D (2007) Effect of nanotube functionalization on theproperties of single-walled carbon nanotube/polyurethane composites. J Polym Sci Part BPolym Phys 45:490–501
Sun L, Warren GL, O’Reilly JY, Everett WN, Lee SM, Davis D, Lagoudas D, Sue HJ et al (2008)Mechanical properties of surface-functionalized SWCNT/epoxy composites. Carbon46:320–328
Zhang ZQ, Liu B, Chen YL, Jiang H, Hwang KC, Huang Y (2008) Mechanical properties offunctionalized carbon nanotubes. Nanotechnology 19:395702
Kuang YD, He XQ (2009) Young’s moduli of functionalized single-wall carbon nanotubes undertensile loading. Compos Sci Technol 69:169–175
Ling CC, Xue QZ, Zhou XY (2012) Mechanical properties of functionalized carbon nanotube asreinforcements. Adv Mat Res 583:22–26
Milowska KZ, Majewski JA (2013) Elastic properties of functionalized carbon nanotubes. PhysChem Ch Ph 15:14303–14309
Ponder JW (2000) Washington University in St. Loius, St. LouisAllinger NL, Yuh YH, Lii JH (1989) Molecular mechanics. The MM3 force field for
hydrocarbons. J Am Chem Soc 111:8551–8566 (and subsequent papers)Volpe M, Cleri F (2003) Chemisorption of atomic hydrogen in graphite and carbon nanotubes.
Surf Sci 544:24–34Letardi S, Celino M, Cleri F, Rosato V (2002) Atomic hydrogen adsorption on a Stone-Wales
defect in graphite. Surf Sci 496:33–38Weininger D (1988) SMILES, a chemical language and information system. 1. Introduction to
methodology and encoding rules. J Chem Inf Comput Sci 28:31–36Weininger D, Weininger A, Weininger JL (1989) SMILES. 2. Algorithm for generation of unique
SMILES notation. J Am Chem Soc 29:97–101
134 P. H. Shah and R. C. Batra